From molybdenum based model catalysts to technically applied systems
Stefan Knoblaus Selb
Fakultt II - Mathematik und Naturwissenschaftender Technischen Universitt Berlin
zur Erlangung des akademischen GradesDoktor der Naturwissenschaften
Dr. rer. nat.
Vorsitzender: Prof. Dr. rer. nat. R. SchomckerBerichter/Gutachter: Prof. Dr. rer. nat. M. LerchBerichter/Gutachter: Prof. Dr. rer. nat. R. Schlgl
Tag der wissenschaftlichen Aussprache: 09. Mrz 2004
I would like to express my gratitude towards all my colleagues in the AC department
for a good working atmosphere and support.
Thanks to the team in Kuala Lumpur, especially Norli, Diana and Q. and Prof. Dr.
Sharifah B. Hamid.
Thanks to the team in Novosibirsk, especially Galina A. and Galina N.
I would like to thank especially Olaf for his guidance and his readiness to discuss all
kind of things. Further, I would like to thank Pablo and Gisela.
I would like to thank Prof. Dr. M. Lerch for the report, and Prof. Dr. R. Schomcker
for being the chairman.
Further, I am in debt to Dr. G. Mestl for the first supervising part.
Thanks to Dr. D. Niemeyer for supervising the second part and for his guidance.
Finally I would like to thank Prof. Dr. R. Schlgl for putting up with me, for his
support, his ideas, his readiness to discuss and for the good working conditions.
Many thanks to my parents and to Brbel.
Table of contents
From molybdenum based model catalysts to technically applied systems 11 Introduction 11.1 General Introduction 11.2 Mo-only model systems 31.3 Multi Metal Oxides 52 Controlled preparation of molybdenum oxide catalysts 102.1 Introduction 102.2 Experimental 12Preparation 12XRD 13TEM 13Raman DRIFTS 13UV/Vis/NIR 13BET 14TG 14TPRS 142.3 Results 142.3.1 Orthorhombic MoO3 15pH-dependency 16XRD 16Raman 16DRIFTS 16UV/Vis NIR 17Thermal analysis 17TPRS 182.3.2 Trimolybdate 18pH dependency 18XRD 18Raman 20DRIFTS 20UV/Vis/NIR 21Thermal Analysis 212.3.3 Hexagonal MoO3 21pH dependency 22XRD 23Raman 24DRIFTS 24UV/Vis/NIR 25Thermal Analysis 26SEM/TEM 28TPRS 292.3.4 Mo36O1128- supramolecular molybdenum oxide 30pH dependency 32XRD 32Raman 32DRIFTS 33UV/Vis NIR 33Thermal Analysis 34SEM/TEM 36
TPRS 372.3.5 Up scaling 38Preparation and pH-dependency 38Electron Microscopy and Electron Diffraction 38TPRS 392.4 Discussion 412.4.1 Effect of counter cation 432.4.2 Effect of temperature and proton to molybdenum ratio 442.4.3 Effect of water 452.4.4 Structure determination by XRD and TEM 472.4.5 Raman and DRIFTS 502.4.6 TPRS 512.5 Conclusion 532.6 Tables 543 In situ Raman investigation of the decreasing pH preparationmethod leading to various MoO3 structures 743.1 Introduction 743.2 Experimental 75Preparation 75Raman spectroscopy 763.3 Results 763.3.1 Reaction at 30 C 763.3.2 Reaction at 50 C 773.3.2 Reaction at 70 C 783.4 Discussion 793.5 Conclusion 834 Nanoclusters as Precursors to (MoVW)5O14: In situ andchemical characterisationof the systems of a single phase oxidation catalyst 874.1 Introduction 874.2 Experimental 884.3 Results 904.3.1 UV/Vis spectroscopy 904.3.2 Conductivity measurements 924.3.3 95Mo NMR spectroscopy 934.3.4 ESR spectroscopy 964.4 DISCUSSION 974.5 CONCLUSIONS 1005 The Synthesis and Structure of a Single Phase, NanocrystallineMoVW Mixed Oxide Catalyst of the Mo5O14-Type 1055.1 Introduction 1055.2 Experimental 1075.3 Results and discussion 1095.3.1 SEM 1095.3.2 Particle size distribution and BET surface area 1105.3.3 TG-MS 1105.3.4 XRD 1125.3.5 HRTEM 1165.3.6 Raman Spectroscopy 1195.3.7 Catalytic properties 123
5.4 Conclusion 1266 Conclusion and Outlook 1336.1 Structure - activity relation 1336.2 Preparation and reactions in solution 1346.3 Outlook 135
From molybdenum based model catalysts
to technically applied systems
1.1 GENERAL INTRODUCTION
About one quarter of added value world wide is produced via catalytic reactions that
originate from partial oxidation reactions and contribute to the gross national product
of industrialised countries. Many catalytic systems are based on molybdenum
oxides. Common reactions are the partial oxidation of propane, propene and acrolein.
The availability and price of the feed stock mentioned above depend largely on
economic conditions, caused by changes in refinery technique, resources (natural
gas) and political interests in oil producing countries. Propane however needs
different catalysts e.g. a molybdenum based catalyst with vanadium, tellurium and
niobium (MoVTe) for partial oxidation reactions[1;5;6], whereas the acrolein oxidation
is carried out on V and W promoted Mo suboxides[2-4]. Test reactions in this thesis
were the partial oxidation of propene (first part) and the partial oxidation of acrolein
High performance catalysts have been developed for these reactions and optimised
by empiric methods. High throughput experimentation (precipitation and testing) is
very successfully applied for development and testing of high performance systems.
However many important details are not monitored by this approach. Effects caused
by minor amounts of additives cannot be precisely recorded. Further parameters
which are often considered to be minor but decisive for the preparation are the speed
of addition, concentrations of precursor solutions, concentration gradients, speed of
stirring, type and form of stirrer, temperature, size of the reaction vessel, solubility,
super-saturation, rate of precipitation, mode of operation and mixing sequence. These
influences are difficult to control and to elaborate in detail scientifically in such
experiments. The major disadvantage of high throughput experimentation (hthe) is
that it does not improve the understanding of the chemistry behind the preparation
process. Consequently high throughput experimentation is most effective with a
knowledge based support and knowledge based key experiments.
Only a knowledge based approach will make straightforward developments of new
processes possible and improve industrial catalysts. The ultimate goal of this work
was to contribute to the fundamental understanding of partial oxidation catalysis i.e.
to understand the function of a catalytically active material. One step towards this
goal was the identification of a structure reactivity relation. Suitable model catalysts
have been prepared because industrial systems are both structurally and chemically
In order to rationalise and explain catalytic reactions various theories are discussed in
the literature such as spill over phenomena, site isolation and phase cooperation [1;16;17]. To test these theories and to generate more knowledge about catalytic
reaction mechanisms the focal point of this thesis was to provide well defined
materials with varying degrees of complexity.
Structural Inorganic Chemistry was a good starting point for the development of
preparation strategies for larger scale functional materials such as catalysts based on
the paradigm of a principle structure-reactivity relationship. In order to be a useful
candidate for a model catalyst more than just the structural information is necessary.
Relevant for catalysis is the `real structure of the material. This includes knowledge
about nanostructuring, particle size, composites, surface phenomena and amorphous
parts. Only after having gained thorough information about this structurally complex
systems and the influence of the addition of vanadium and tungsten can be
understood (chapter 4 and 5).
This enables a knowledge based approach of catalyst preparation and the specific
improvement of catalytic properties. This can be seen as an iterative improvement
starting with well defined and documented preparation and activation. After a
thorough ex- and even more important in situ characterisation of the material the
second iterative cycle started with the preparation of the identified active phases in a
pure form. Having this well characterised material in hand a structure reactivity
relation was established which was refined in the following cycles.
This strategy enabled generation of information about industrially relevant processes
under realistic conditions (e.g. reaction temperature and pressure). The obtained
material was more similar to the industrial catalysts than single crystals applied in
UHV and surface science studies but still well defined enough for scientifically
valuable conclusions. Consequently the results are relevant for industrial multi
million ton processes.
1.2 MO-ONLY MODEL SYSTEMS
Structural changes of molybdenum species in solution were investigated as a
function of pH under preparative conditions. Precursors such as ammonium hepta
molybdate (AHM), sodium molybdate (Na2MoO4), lithium molybdate (Li2MoO4)
and potassium molybdate (K2MoO4) were dissolved in water. The pH was decreased
by adding HNO3. Precipitation led to solid catalyst precursor. Another method
applied to obtain a solid was spray drying[18; 19].
Depending on the preparation conditions the molybdenum oxygen systems
developed structures which were also identified in high performance catalysts used in
production plants. A hexagonal molybdenum oxide phase showed a structure similar
to the M 2 phase of the MoVTeNb system used industrially for the partial oxidation
of propane[1;16;17;21-24]. Other authors found the same structure and named it
Another example is Mo5O14 which is identified as active phase of an industrial
MoVW Oxide catalyst for the selective partial oxidation of acrolein or propene to
acrylic acid. The characteristic structural motif is a pentagonal bipyramid. This motif
is also found in Mo36O1128-. Therefore the model system allows studying structurally
highly complex materials with low chemical complexity.
The complex parameter space such as temperature, molybdenum concentration, and
acid concentration was investigated with an automated titration machine which is an
excellent tool for fast screening. The influences of up scaling were examined with a
reaction vessel one order of magnitude larger than the titrator.
One important aim of chapter two was further to bridge gaps between Structural
Inorganic Chemistry in aqueous solution and Solid State Chemistry and further
between Solid Phase Chemistry and functional materials.
Very early investigations on aqueous molybdenum systems were carried out[18; 19].
The main methods used at this time were determination of diffusion coefficients,
UV/Vis and conductometric-, potentiometric-, and thermometrictitrations. Saski
and Sillen presented the first comprehensive potentiometric investigation. A
milestone was the identification of the hepta and octa molybdate structures by X-ray
single crystal analysis[26-28].
Significant contributions were made by Aveston and Anacker and also by Tytko and
Glemser[29-37]. They combined Raman spectroscopy and single crystal analysis,
which enabled them to compare solid state structures with compounds in solution.
Contributions to reveal details of the reaction mechanism were delivered by O-NMR
spectroscopy[38-40]. Recently Cruywagen published more potentiometric data and a
computer aided evaluation[41-43]. All experiments were carried out at room
temperature with diluted solutions.
With the help of these data four different structures were obtained on a preparative
scale. Using TEM it was shown that so called `minor species in solution obviously
play an important role in the solidification process. Therefore the role of integral
analytical techniques such as Raman spectroscopy and XRD were reflected critically.
One task of this work was to test whether this knowledge is applicable under
preparative conditions. This was achieved by carefully controlling parameters such
as pH, conductivity, temperature etc. in small and large scale reactions. To bridge the
above described gaps the solid phase chemistry of the obtained catalyst precursors
was investigated by TG/DSC-MS and the catalytic behaviour was monitored by
temperature programmed reaction spectroscopy (TPRS).
1.3 MULTI METAL OXIDES
The second part of this work was dedicated to the more complex system
(Mo0.68V0.23W0.09)5O14. Based on the knowledge generated by using the model
systems a single crystalline phase was obtained. This procedure was investigated by
a variety of analytical techniques such as in situ Raman spectroscopy, pH-
measurements, conductivity-measurements and UV/Vis spectroscopy. In order to
follow the preparation in detail a novel in situ method was developed for UV/Vis
measurements based on a reflection fibre optic.
The reaction mechanism that has been set up for the binary model system was in
principle transferred to the complex system. The role of vanadium was identified as
the linking element between isomerising octamolydate species.
From the catalytic point of view it was shown that the very ill defined phase mixture
in the industrial catalyst can be reduced to only one catalytically relevant crystalline
phase, namely Mo5O14. Additional phases are most likely just side products of the
However, it was shown that a single crystalline phase theory is too simple to explain
the whole catalytic process as differences in catalytic activity were detected with
compounds of identical stoichiometry and XRD pattern. Similar to the model case
amorphous overlayers were detected on the single phase material. Therefore the
approach to control the real- and nano structure is much more important than the
influence of additives.
Comparing this thesis to traditional catalyst research and optimisation it is striking
that almost only additives are changed. Here however a novel approach is presented.
Carefully chosen model catalysts which contain only molybdenum and oxygen were
described. Several reasons support this choice. Firstly, much catalytic data is
available on orthorhombic MoO3. This has been reviewed lately by Haber[44-46].
Secondly, as nanostructuring oxygen mobility and vacancies are considered to play a
major role in catalysis (Mars van Krevelen) molybdenum oxides are good candidates
for investigation. Related to this are substoichiometric oxides so called Magneli
phases[47-55]. Therefore on the one hand this work is the logical consequence of
preceding work carried out in this department on molybdenum oxides e.g. three
preceding Ph.D. theses by Dieterle, Wienold and Blume and numerous
publications[11;15;59;60]. On the other hand this preparative approach opens the way to
check recent theories on tailor like materials.
Additionally molybdenum oxides are very sensitive to changes of the preparation
conditions. Therefore an investigation of this system is absolutely needed. The role
of additives can only be understood after the effects of the matrix are known
[1.] R. K. Grasselli, Catal.Today 1999, 49 141-153.
[2.] Hibst, H. and Unverricht, S. BASF AG. [DE 19815281 A 1]. 1981.
Ref Type: Patent
[3.] Hibst, H. and Unverricht, S. BASF AG. [DE 19815281 A 1]. 1981.
Ref Type: Patent
[4.] Tenten, A., Martin, F.-G., Hibst, H., Marosi, L., and Kohl, V. BASF AG. [EP 668104 B1].
Ref Type: Patent
[5.] R. K. Grasselli, J. D. Burrington, Advances in Catalysis 1981, 30 133.
[6.] R. K. Grasselli, Surface Reaktion Mechanisms of Selective Olefin Oxidation over Mixed
Metal Oxides, (Eds.: M. Che, G. C. Bond) Elsevier, Amsterdam 1985, p. 275.
[7.] Kurtz, A. N., Cunningdam, R. W., and Naumann, A. W. Union Carbide Co. [US 4111983].
Ref Type: Patent
[8.] Novak, V., Sokol, L., and Jelinek, J. CS1207807B. 1981.
Ref Type: Patent
[9.] Bertolini, N. and Ferlazzo, S. Euteco Impianti S.p.A. [US 4289654]. 1981.
Ref Type: Patent
[10.] Kawajiri, T., Uchida, S., and Hironaka, H. Nippon Shokubai Kagaku. [EP 427 508 A1].
Ref Type: Patent
[11.] M. Dieterle, G. Mestl, J. Jger, Y. Uchida, R. Schlgl, J.Mol.Catal.A: Chemical 2001, 74
[12.] M. Dieterle, G. Mestl, Phys.Chem.Chem.Phys. 2002, 4 822.
[13.] S. Knobl, G. A. Zenkovets, G. N. Kryukova, O. Ovitser, M. Dieterle, R. Schlgl, G. Mestl,
J.Catal. 2003, 215 177-187.
[14.] G. Mestl, Ch. Linsmeier, R. Gottschall, M. Dieterle, J. Find, D. Herein, J. Jger, Y. Uchida,
R. Schlgl, Journal of Molecular Catalysis 2000, 162 455-484.
[15.] T. Ressler, O. Timpe, T. Neisius, J. Find, G. Mestl, M. Dieterle, R. Schlgl, Journal of
Catalysis 2001, 191 75-85.
[16.] R. K. Grasselli, Topics in Catalysis 2001, 15 93.
[17.] R. K. Grasselli, Topics in Catalysis 2002, 21 79.
[18.] G. Jander, K. F. Jahr, W. Heukeshoven, Zeitschrift fur Anorganische und Allgemeine Chemie
1930, 194 383-428.
[19.] A. Rosenheim, Zeitschrift fur Anorganische und Allgemeine Chemie 1916, 96 139.
[20.] B. Krebs, I. Paulat-Bschen, Acta Cryst. 1976, B32 1697.
[21.] Hatano, M. and Kayou, K. [EP 318295]. 1988.
Ref Type: Patent
[22.] T. Ushikubo, K. Oshima, A. Kayou, M. Hatano, Study of Surface Science and Catalylis,
(Eds.: C. Li, Q. Xin) Elsevier, Amsterdam 1997, p. 473.
[23.] M. M. Lin, Applied Catalysis A-General 2003, 250 305-318.
[24.] M. M. Lin, Applied Catalysis A-General 2003, 250 287-303.
[25.] Y. Sasaki, L. Silln, Arkiv Fr Kemi Mineralogi och Geologi 1968, 29 253.
[26.] I. Lindquist, Arkiv Fr Kemi Mineralogi och Geologi 1950, 18 325-341.
[27.] I. Lindquist, Arkiv Fr Kemi Mineralogi och Geologi 1950, 2 349.
[28.] I. Lindquist, Acta Cryst. 1950, 3 159.
[29.] J. Aveston, E. W. Anacker, J. S. Johnson, Inorganic Chemistry 1964, 3 735-746.
[30.] I. Bschen, B. Buss, B. Krebs, O. Glemser, Angew.Chem. 1973, 85 409.
[31.] O. Glemser, W. Holznagel, A. Iftikhar, Z.Naturforsch. 1965, 20b 192.
[32.] K.-H. Tytko, B. Schnfeld, B. Buss, O. Glemser, Angewandte Chemie 1973, 85 305-307.
[33.] K.-H. Tytko, B. Schnfeld, Zeitschrift fur Naturforschung 1975, 30b 471-484.
[34.] K.-H. Tytko, O. Glemser, Adv.in Chem.Series 1976, 19 239-315.
[35.] K.-H. Tytko, O. Glemser, Adv.Inorg.Chem.Radiochem 1976, 19 239.
[36.] K.-H. Tytko, G. Baethe, E. R. Hirschfeld, K. Mehmke, D. Stellhorn, Z.Anorg.Allg.Chem.
1983, 503 43-66.
[37.] K.-H. Tytko, G. Baethe, Z.Anorg.Allg.Chem. 1987, 555 85-97.
[38.] V. W. Day, M. F. Fredrich, W. G. Klemperer, W. Shum, J.Am.Chem.Soc. 1977, 99 6146.
[39.] W. G. Klemperer, W. Shum, J.Am.Chem.Soc. 1976, 98 8291.
[40.] W. G. Klemperer, Angew.Chem. 1978, 17 246.
[41.] J. J. Cruywagen, J. B. B. Heyns, Inorganic Chemistry 1987, 26 2569.
[42.] J. J. Cruywagen, Advances in Inorganic Chemistry 2000, 49 127.
[43.] J. J. Cruywagen, A. G. Draaijer, J. B. B. Heyns, E. A. Rohwer, Inorganica Chimica Acta
2002, 331 322.
[44.] J. Haber, Catalysis by Transition Metal Oxides, (Eds.: R. Grasselli, J. Brazdil) American
Chemical Society, Washington D. C. 1985, p. 1.
[45.] J. Haber, 3 rd World Congress on Oxidation Catalysis, (R.K.Grasseli, S.T.Oyama,
A.F.Gaffney, J.E.Lyons) 1997, 1997 Elsevier, Amsterdam 1.
[46.] J. Haber, V. Turek, Journal of Catalysis 2000, 190 320-326.
[47.] G. Andersson, A. Magnli, Acta Chemica Scandinavica 1950, xxx 793-797.
[48.] A. Magnli, Arkiv Fr Kemi Mineralogi och Geologi 1946, 24 a 1.
[49.] A. Magnli, Acta Chemica Scandinavica 1948, 2 501-517.
[50.] A. Magnli, Acta Chemica Scandinavica 1948, 2 861-871.
[51.] A. Magnli, G. Andersson, B. Blomberg, L. Kihlborg, Analytical Chemistry 1952, 24 1998.
[52.] A. Magnli, Research 1952, 5 394.
[53.] A. Magnli, Acta Cryst. 1953, 6 495.
[54.] A. Magnli, G. Andersson, Acta Chemica Scandinavica 1955, 9 1378-1381.
[55.] A. Magnli, B. Blomberg-Hansson, L. Kihlborg, G. Sundkvist, Acta Chemica Scandinavica
1955, 9 1382.
[56.] Dieterle, M., TU Berlin, 2000.
[57.] Wienold, J., 2003.
[58.] Blume, A., TU Berlin, 2004.
[59.] M. Dieterle, G. Mestl, Phys.Chem.Chem.Phys. 2002, 4 822.
[60.] O. Ovitser, Y. Uchida, G. Mestl, G. Weinberg, A. Blume, J. Jager, M. Dieterle, H. Hibst, R.
Schlgl, J.Mol.Catal.A: Chemical 2002, 185 291-303.
2 Controlled preparation of molybdenum
The production of high value petrochemicals such as acrolein or acrylic acid is carried
out by selective oxidation of lower alkanes over molybdenum oxide based catalysts[1-9].
Empirical optimisation of the catalyst performance through doping with foreign cations
has already reached a high level again stressing the huge potential of such catalysts.
There is a number of recent patents for a material with the approximate composition of
Mo1V0.33Te0.22Nb0.11Ox[10-15]. Characterisation of this material has led to the
identification of two major phases amongst other minor phases. The first one (M1) is
orthorhombic and isostructural of Cs0.7(NbW)5O14 and shows a great similarity to
Mo5O14 because of its pentagonal bipyramides as the most striking feature. The second
phase (M2) is pseudo hexagonal and isostructural to Sb4Mo10O31.
Although additives are proven to enhance catalytic activity there is an ongoing debate
about whether they act as structural builders or linkers and therefore favour a certain
type of structure or they form active sites themselves. Grasselli[17-19] has outlined `seven
pillars of selective oxidation, in which `phase cooperation and site isolation are two of
his major concepts. As testing these concepts on multi component and multi phase
industrial catalysts is rather difficult, there is a need for good model catalysts. A
breakthrough was achieved recently by the successful synthesis of single phase
(MoVW)5O14 material. This synthesis was done with a nanostructured precursor as
intermediate in which vanadyl linkers connect octamolybdate species, that were
distorted by tungsten atoms. During the catalytic reaction at elevated temperature the
material undergoes structural and electronic changes and its activity and selectivity are
enhanced. The post mortem sample shows the Mo5O14-type structure, which was first
discovered by Kihlborg. This work led to the conclusion that the function of V and
W atoms is only to form and stabilise the catalytically active site of Mo5O14. This
assumption would be further validated, if a solid containing such sites would be
successfully prepared containing only molybdenum and oxygen. This material should
then have a similar catalytic activity to the industrial (MoVW)5O14 catalyst.
Another matter of debate is whether the catalytic reaction happens on bulk-terminated
oxide, as can be deducted from Grassellis work, or on differently coordinated Mo oxide
surface layers. The latter statement can be supported by studies from Wachs et al. who
investigated methoxy chemisorption on monolayer supported Mo oxide prepared by
incipient wetness. They found a correlation between the monolayer of methoxy
species of the surface and the number of active surface sites. These sites were formed by
transformation of crystalline (bulk) metal oxides into active surface metal oxide species
by reaction-induced spreading. This phenomenon clearly depends on the nature of the
support. Bell et al. identified the active surface species as two dimensional MoOxpolymers, who are favoured at low surface densities
variables have been reported in earlier work, dealing with pH dependent reactions of
Mo compounds in aqueous solution[36-38] [39-46] [47-50] [51;52]   [52;54-62] [63-66] [67-69].
These variables are extrapolated on a preparative scale in order to ensure the production
of different structural families. Clusters containing these pentagonal bipyramides should
show catalytic activity without any need for calcination or activation, as these
procedures cause uncontrolled reformation of the clusters, leading to pure ortho-MoO3revealed in its defect-free form, if the temperature is raised above 500 C. This material
shows unsuitable local chemical bonding for selective oxidation[9;70-72] and requires
tuning by the introduction of defects that can be achieved by heating the sample above
the limit of oxygen diffusion to the surface. Finally up scaling is an important factor to
ensure a reproducible production of catalytic material especially when diffusion plays
an important role in the reaction mechanism.
All solids were obtained by precipitation. Small-scale preparation (200 ml) to scan the
parameter range was carried out in a Mettler-Toledo DL 77 Titrator to which an
automated Rondo 60 sample changer was attached. The Rondo was modified in such a
way that a water bath maintained constant temperature conditions. As starting material
aqueous solutions of (NH4)6Mo7O24 * 4 H2O (AHM), Na2MoO4, Li2MoO4, K2MoO4 (all
MERCK, p.a.) at a concentration range between 0.28 mol/l and 2 mol/l calculated on
Mo was used. As precipitation agent HNO3 (1 mol/l 5 mol/l) was applied. The
experiments were carried out at 30 C, 50 C and 70 C.
In a separate set of experiments the effects of up scaling have been studied by using a
home-made 4l computerised semi-technical preparation set-up allowing to control the
temperature accurately and to measure pH and electrical conductivity. The same
concentration ranges have been used as before, the starting solution was 1l. The pH and
was recorded and analyzed digitally. After the addition of HNO3 the samples were
allowed to age for 1 h at 35 C. All samples were filtered and dried in a desiccator over
dry gel. It is crucial not to wash the samples, as this would cause partial re- dissolution.
A STOE STADI-P focusing monochromatic transmission diffractometer equipped with
a Ge(111) monochromator and a position sensitive detector. Cu-Ka radiation was used.
The phase analysis was performed with the STOE Win XPOW software package
(version 1.06; Stoe Darmstadt, Germany) and with PowderCell (V 2.3; Bundesanstalt
fr Materialforschung und -prfung (BAM) Berlin, Germany).
The samples were prepared for transmission electron microscopy (TEM) by standard
preparation routines. The powder is suspended in ethanol and dispersed onto a standard
meshed copper grid coated with a holey carbon film, by dipping the grid into the slurry.
The samples are studied in a Philips CM 200 FEG electron microscope operated at
200~kV and equipped with a Gatan Image Filter and a CCD camera. Scanning electron
microscopy (SEM) images are acquired with an S 4000 FEG microscope (Hitachi).
Raman spectroscopy was performed on a Labram I (Dilor) instrument equipped with a
confocal microscope (Olympus). A notch filter (Kaiser Optical) was applied to cut off
the laser-line and the Rayleigh scattering up to 150 cm1. The spectrometer is equipped
with a CCD camera (1024*298 diodes), which is Peltier cooled to 30 C to reduce the
thermal noise. A He-laser (Melles Griot) was used to excite the Raman scattering at 632
nm with a laser power of 1,4 mW. The following spectrometer parameters were used:
microscope objective: 10; slit width: 200 m (spectral resolution: 2.5 cm-1), integration
time: 30 s per spectrum and 5 averages.
DRIFTS were recorded on a Bruker ifs 66 FTIR-spectrometer equipped with OPUS
software. 100 spectra were averaged and the resolution was 4 cm-1. The spectra were
recorded in air. For background measurement KBr was used. The aperture was set to 5
mm, scan velocity 7; 20 kHz.
A commercial UV-Vis-NIR spectrometer (Lambda 9, Perkin Elmer) equipped with an
integrating sphere was supplemented with a construction to measure in situ diffuse
reflectance spectra from room temperature to 450 C. A full description of the complete
setup has been given elsewhere.
BET was carried out on a Quantachrom Autosorb-1 apparatus. Degassing of the sample
was carried out at 120 C for two hours. 0.3 g of sample was weighed in and nitrogen
was used as adsobate.
Thermal analysis (TA) was performed with a STA 449 C Jupiter apparatus (Netzsch).
Flowing helium and air atmosphere were applied (the flow rate was set at 15 ml/min in
both cases). The heating rate was set at 5 C/min. Mass spectrometric analysis (TG-MS)
of the evolved gases was performed with an Omnistar quadrupole mass spectrometer
The test reaction for TPRS was the partial oxidation of propene. The instrumentation for
the TPRS runs consists of a simple tubular reactor. The sample (50 mg) is diluted in a
matrix of BN and SiC (for amelioration of heat transfer).
The total gas flow is set to 100 ml/min and the resulting hsv ranges about 13500. The
feed is composed of 10 % propene and oxygen each in He. The temperature is ramped
twice to 500 C by 5 C/min in two successive cycles.
Depending on preparation conditions such as temperature, molybdenum concentration,
acid concentration and the choice of starting material and counter ion such as Li+, Na+,
K+, NH4+ four different families of products were obtained by precipitation:
orthorhombic MoO3, hexagonal MoO3, trimolybdate and a supramolecular Mo36O1128-
like compound (Fig. 2.1).
2.3.1 Orthorhombic MoO3
Orthorhombic MoO3 is only obtained with Li+ as counter ion. Regardless of the
preparation temperatures further heating to the boiling point was necessary to force
Lithium monomolybdate shows typically an initial pH at around 6.5 (Fig. 2.2).
Acidification with nitric acid leads first to a sudden pH drop followed by a buffering
region around pH = 5.5 and a further drastic pH drop down to pH = 2. This pH curve is
very temperature dependent as the sample treated at 50 C needs the smallest amount of
acid in this series to reach its final pH = 1. The second largest acid volume is used for
the sample at 70 C. The 30 C sample needs the largest amount of acid. In Fig. 2.2 the
amount of acid added is normalised to the acid concentration and to the molybdenum
concentration. Therefore all pH data shown in this plot can be directly compared.
Figure 2.1: Lead structures of the obtained materials identified by XRD and
Raman; a) supramolecular compound; b) hexagonal MoO3; c) trimolybdate;
d) orthorhombic MoO3
All three samples show the pattern of orthorhombic MoO3 however poorly crystalline.
One typical pattern is shown in Fig. 2.4 B (222). The indexing was done according to
Bands are detected at 996, 825, 667, 376, 335, 292 and 244 cm-1. This is in line with the
bands reported in the literature for orthorhombic MoO3 apart from the band at 825
cm-1, which should be at 820 cm-1. Further a shoulder is detected at 980 cm-1, which
does not belong to MoO3. Fig. 2.5 (222) shows a typical Raman spectrum, the other
samples are listed in Table 2.6.
Bands are found at 840, 743, 1000, 1387, 1636, 1946, 2389, 3584 cm-1. The band at
3584 cm-1 is assigned to OH stretching and deformation frequencies of hydrated water
respectively. The band at 1636 cm-1 suggests that water is present as water molecules as
well as hydroxyl[75-77]. Representative spectra are shown in Fig. 2.9 and 2.10.
0,0 0,2 0,4 0,6 0,8 1,0 1,2 1,4
7251 30 C222 50 C230 70 C
Figure 2.2: pH curve for samples (LiMoO4 0.28 mol/l HNO3 2 mol/l) 251,
30 C; 222, 50 C; 230, 70 C. Data normalised to molybdenum and acid
Bands in the NIR region are detected at 1430, 1790, 1930 and 2280 nm as seen in Fig.
2.25. The sample prepared at 50 C shows the biggest band areas and a band gap energy
of 3.37 eV. The band gap energy of the other two samples is 3.48 eV (Fig. 2.7 I, II).
Results are listed in Table 2.4. A strong band at 970 nm is observed in the samples
prepared from 0.28 mol/l Li2MoO4 with 2 mol/l HNO3 at 30 oC and 50 oC. Such a band
cannot be observed for all other samples with hexagonal MoO3, supramolecular
Mo36O1128-, and trimolybdate structure as can be seen in Fig. 2.13.
Although precipitation was only achieved after boiling of the aqueous solutions, the
precipitation temperature seems to have an effect on the behaviour during calcination.
The sample (Fig. 2.3; 222) prepared at 50 C shows the most characteristic events in the
TG-MS. The biggest overall mass loss is detected for the sample prepared at 50 C (7
%) and the last mass loss at 320 C is most pronounced and accompanied by a
significant endothermic signal. This sample shows a peak in the water signal (MS) at 75
C. After that water is evolved constantly up to 240 C. NOX at 320 C is evolved. The
intensity of the water signal is nicely reflected by the DSC trace. The maximum of the
water MS trace coincides with a minimum in the DSC curve. As soon as the water MS
trace is declining the DSC curve is getting steeper.
Relative to the other two samples the NOX signal is much bigger. The TG traces of the
samples prepared at 30 C and at 70 C are similar showing an almost constant mass
100 200 300 400 50090
Figure 2.3: TG-DSC of 222, 230 and 243
loss up to 266 C and hardly any mass loss up to appr. 310 C. From 372 C upwards no
more mass losses are detected. Some decisive differences however appear in the DSC
trace. The sample prepared at 30 C shows an exothermic transition at 238 C which
coincides with the declining water MS trace. As soon as no more water is present the
DSC trace is changing its curvature. An endothermicity is detected at 352 C at the
same time NOX is evolved. In contrast to that the sample prepared at 70 C shows a
plateau in the DSC curve at 311 C. From this temperature on no more water is evolved.
At 330 C water is leaving the sample.
The obtained orthorhombic MoO3 starts to convert propene to CO2 at around 300 C. At
350 C a plateau is reached. Another rise in activity is observed at 370 C and at 430 C
the maximum CO2 production is measured (Fig. 2.20 and 2.21).
Trimolybdate is obtained with K+ as counter ion and at a reaction temperature of 70 C
and a minimum molybdenum and acid concentration of 2 mol/l. In this investigation
trimolybdate was obtained with K2MoO4 2 mol/l, HNO3 2 mol/l and 5 mol/l. The
compound precipitates spontaneously (sample 244 and 243).
The titration starts at around pH = 9, buffers at around pH = 7 and reaches the final pH
= 1 asymptotically (Fig. 2.18).
Using K2MoO4 2 mol/l and HNO3 2 mol/l the XRD pattern (Fig. 2.4, sample 243)
indicates a phase mixture containing hexagonal MoO3, trimolybdate and at least one
more phase. The interpretation is difficult because peaks can shift depending on the
It is reported[46;78] that cation spaces could be either occupied by H3O+ or K+. Depending
on this crystal parameters will change. However, it cannot be ruled out that more phases
are present. Increasing the acid concentration increases the amount of trimolybdate.
Figure 2.4: A XRD pattern of representative samples. 256, supramolecular
phase from AHM; 227, hexagonal MoO3 from AHM; 229, hexagonal MoO3from K2MoO4; 243, supramolecular from K2MoO4;
B 222, orthorhombic MoO3 from Li2MoO4; 245, supramolecular compound
10 20 30 40 50 60 70
10 20 30 40 50 60 70
The main bands are observed at 949, 938, 909, 612, 372 and 217 cm-1. Taking the
intensity pattern into account it fits with the literature values reported for K2O * 3 MoO3* x H2O (Fig. 2.5). However there is a slight, non-systematic shift in band positions. In
the literature a triad of very sharp bands is reported. This triad is not well resolved when
HNO3 2 mol/l is used as precipitation agent and a further shoulder is detected at 873 cm-
1, which is not reported in the literature. The band detected at 1051 cm-1 is assigned to
nitrate from the precipitation agent. Again an increase of the acid concentration leads to
a purer product and the band positions fit exactly with the ones reported in the literature.
Bands are detected at 726, 804, 880, 955, 1337, 1447, 1633, 2170, 2383, 2754, 3298,
3532 cm-1. The assignment of the water bands corresponds to the one done above for
the orthorhombic MoO3. At lower wavenumbers different bands are detected. Therefore
IR can discriminate among these compounds (Fig. 2.9 and 2.10).
1000 800 600 400 200
Raman shift (cm-1)
Figure 2.5: Raman spectra of representative samples. 256, supramolecular
phase from AHM; 227, hexagonal MoO3 from AHM; 229, hexagonal MoO3from K2MoO4; 245, supramolecular from K2MoO4; 243, trimolybdate; 222,
NIR bands are detected at 1435 and at 1935 nm with quite low intensity. In addition two
weak bands at 1790/1810 nm and stronger bands at 2000, 2095 and 2250 nm were
detected. Besides a small LMCT centred at 284 nm and an Eg of 3.77 eV are observed
(Table 2.4). The band gap energy in the sample prepared from 2 mol/l K2MoO4 with 2
(5) mol/l HNO3 at 70 oC is 3.77 eV. The sample prepared from the higher concentrated
acid (5 mol/l) shows a band gap energy of 3.77 eV.
Trimolybdate (Fig. 2.3, sample 243) reaches mass constancy at 130 C. At this
temperature a sharp endothermic signal is detected. A further endothermic signal
appears at 333 C. At around 420 C the samples start to melt. The two samples do not
show any decisive differences.
2.3.3 Hexagonal MoO3
Hexagonal MoO3[79-82] is obtained with Na+, K+ and NH4+ as counter ion. It is either
obtained by spontaneous precipitation at higher temperatures or by further heating of the
100 200 300 400 50092
Temperature / oC
Figure 2.6: TG-DSC of 219, 229 and 227
solution at pH = 1 to the boiling point. Finally hexagonal MoO3 is only obtained from
rather dilute molybdenum stem solutions.
Employing Na+ as counter ion and a molybdenum and acid concentration of 2 mol/l
respectively no reaction temperature yielded hexagonal MoO3 spontaneously. After
heating hexagonal MoO3 was obtained (samples 252, 226, 255 and 231).
Potassium as counter ion yielded hexagonal MoO3 when the molybdenum concentration
was 0.28 mol/l and HNO3 2.0 mol/l for the reaction temperatures 50 C and 70 C only
after further heating (samples 219, 229, 247 and 233).
Ammonia as counter ion yielded hexagonal MoO3 with an AHM concentration 0.7
mol/l (Mo) and HNO3 1 mol/l at 50 C and at 70 C after further heating (samples 227,
232 and 248).
Using Na+ as counter ion the starting pH is 8.2 for the reaction at 30 C (Fig. 2.8).
Adding 2 mol/l HNO3 leads to a pH drop. At around pH = 7.5 a buffering sets in, which
is followed by a large pH drop again down to pH = 1. The other two reaction
temperatures show a similar behaviour, however the starting pH is lower and the first
300 400 500 600 700 8000
2,5 3,0 3,5 4,0 4,50
Photon energy (eV)
Figure 2.7: Spectroscopic characteristics of orthorhombic MoO3, 251, 222
and 230. I. UV/Vis spectra; II. band gap energies Eg
buffering takes place at around pH = 6.8. It is noteworthy that the sample prepared at 50
C needs considerably less acid to reach the final pH. The highest amount of acid is
needed for the sample prepared at 30 C.
In the potassium case the reaction starts at around pH = 7. Buffering occurs at around
pH = 6.5. Apart from that the curve is very similar to the one described above for
Sodium. Again the reaction at 50 C needs considerably less acid (Fig. 2.18).
The reaction is slightly changing with ammonia as counter ion because the starting
compound is now the heptamolybdate ion rather than the mono molybdate ion.
Therefore the reaction starts at around pH = 5.3. After that the pH is dropping fairly
constantly until pH = 2 is reached. At this point the two pH traces separate. The reaction
at 50 C reaches pH = 1 fairly quickly whereas the solution at 70 C shows a stronger
buffering and needs much more acid (Fig. 2.14 and 2.19).
One representative diffraction pattern of the samples prepared from Na2MoO4 is shown
in Fig. 2.4 A indexed according to PDF-39-35 and ICSD-38415. The pattern fits quite
good to the one reported in the literature apart from a decisive broadening of the signal
at 25.5 2 theta and some additional small signals in the region from 49.3 2 theta to 53.3
2 theta and at around 61 2 theta.
Potassium as counter ion produced clearly hexagonal MoO3. The signals however
possesses shoulders, consequently a second phase with different d-spacings might be
present. Ammonia as counter ion yielded a similar result (Fig. 2.4 A).
0,00 0,05 0,10 0,15 0,20 0,25 0,30 0,35 0,40
8 231 70 C226 50 C252 30 C
Figure 2.8: pH curve for samples (Na2MoO4 2 mol/l, HNO3 2 mol/l) 252, 30
C; 226, 50 C; 231, 70 C. Data normalised to molybdenum and acid
The Raman spectra recorded from the hexagonal MoO3 obtained from Na2MoO4,
K2MoO4 and AHM shows bands at 978, 904, 884, 692, 494, 399, 255 and 229 cm-1.
Only minor shifts and changes in band shape occur. Representative spectra are shown in
Depending on the counter ion small changes are observed. The main bands are detected
at around 726, 804, 886, 955, 996 (sh), 1360, 1612, 3305, 3571 cm-1. Especially the
region below 1000 cm-1 does not fit exactly to literature values. However in the
literature it is shown that not only Mo-O bond stretching and bending vibrations are
detected but also H2O liberational motions. Therefore even the band positions in this
region depend on the quantity of water and ammonia. However the main features match
(Fig. 2.9 and 2.10).
1000 900 800 700 600
Figure 2.9: Diffuse reflectance fourier transform spectroscopy (DRIFTS) of
representative samples. 256, supramolecular phase from AHM; 227,
hexagonal MoO3 from AHM; 229 hexagonal MoO3 from K2MoO4; 245
supramoleculart from K2MoO4; 243, trimolybdate; 222, orthorhombic MoO3
Table 2.4 shows the spectroscopic characteristics of samples prepared from 2 mol/l
Na2MoO4 with 2 mol/l HNO3 at 30 C, 50 C and 70 C, which indicated different band
positions depending on temperature. The spectrum of the sample prepared at 30 C
shows a LMCT band at about 320 nm. This band is red shifted by 8 nm in the spectrum
of the sample prepared at 70C and by 12 nm in the spectrum of the sample prepared at
50 C. All three samples have the same Eg values of 3.27 eV (Table 2.4). In addition
these samples exhibit a very similar behaviour in the NIR region. A very strong
absorption band at 1955 nm, a small band at 1430 nm and relatively weak absorption
bands at 1820 and 2280 nm appear, whereas the sample prepared at 70 C leads to a
spectrum with slightly higher band intensities. The spectra in the NIR range recorded of
the compound prepared from Na2MoO4 are very similar, the main bands are detected at
1430, 1820, 1955 and 2280 nm. Whereas the sample prepared at 70 C shows the
biggest band areas. Band gap energies are very similar as well. For all three compounds
3.27 eV are found.
Switching to K+ as counter ion the bands are located at 1435, 1820, 1935, 2090 and
2235 nm. The band gap energy amounts to 3.30 eV.
1000 2000 3000 4000 5000
Figure 2.10: DRIFTS of representative samples. 256, supramolecular
phase from AHM; 227, hexagonal MoO3 from AHM; 229, hexagonal
MoO3 from K2MoO4; 245, supramolecular from K2MoO4; 243,
trimolybdate; 222, orthorhombic MoO3
Finally the NIR bands for the ammonia-containing compound (0.7 mol/l AHM) are
situated at 1440, 1570, 1945, 2040 and 2150 nm. The band gap energy is 3.35 eV for
the hexagonal compound prepared at 50 C and 3.36 eV for the one prepared at 70 C.
Figure 2.11: A) SEM of hexagonal MoO3, 227; B) TEM, 227; C) HRTEM,
227; D) SEM, 130 large scale; E) HRTEM of 130; F) TEM 130
With the sodium-containing compound the 50 C sample is showing the biggest mass
loss (8.5 %) accompanied by a sharp endothermic signal at 350 C (Fig. 2.12). All three
samples show a sharp exothermic signal at 378 C. A sharp endothermic signal is
detected at 307 C for the sample prepared at 30 C and at 50 C. The samples prepared
at 30 C and at 70 C show a broad endothermic signal at 331 C. The sample prepared
at 30 C evolves NOX at 325 C and at 380 C. The 50 C sample shows only one very
large peak at 350 C. The sample prepared at 70 C looses NOX at 340 C and at 380
The potassium containing samples show a similar thermal behaviour. The overall mass
loss of the sample prepared at 70 C is 5 % and it is 6 % of the sample prepared at 50
C. The TG-trace shows a step at around 100 C. In between 190 C and 320 C the
samples prepared at 50 C and 70 C are fairly mass constant and their TG traces run
almost parallel. At temperatures higher than 320 C a rapid mass loss (2 %) sets in
which is related to an exothermic signal in the DSC curve in the case of the sample
prepared at 50 C.
Simultaneously, a trace of water and NOX is detected in the MS. The sample prepared at
70 C does not show a clear step and no characteristic signals in the DSC trace. At
around 350 C the evolution of water and NOX is detected when the final phase
transition to orthorhombic MoO3 sets in. The final phase transition is shifted to lower
temperatures compared to the hexagonal phase prepared with ammonia as counter ion.
100 200 300 400 500
Temperature / oC
Figure 2.12: TG-DSC, sample 226, 231, 232
The compound obtained from AHM exhibit an overall mass loss of 7 %. At 400 C an
exothermic event is recorded coinciding with the evolution of water and NOX and a
small final mass loss (less than 1 %). The mass loss does not show clear steps and the
MS traces water and NOx continuously (Fig. 2.6).
In a separate experiment the sample was heated to the temperature of the exothermic
event and left at this temperature for one hour. During this procedure the sample
transformed into orthorhombic MoO3.
The morphology of sample 227 is studied with SEM. A characteristic SEM of the
sample is shown in Fig. 2.11 A, B, C. The sample consists of regular hexagonal rods
with a length of several m and a diameter ranging from 1-2 m.
500 1000 1500 2000 2500
Figure 2.13: NIR bands of 252, 245, 233, 244, 251
The particles reveal well-defined facets. However, smaller irregular particles are
observed in the size range below 500 nm. The projected morphology of the hexagonal
rods is recognised in TEM images such as Fig. 2.11.
The small particles are observed here as well. As the well-defined hexagonal shaped
rods not are transparent for 200 keV electrons due to the thickness, lattice fringe
imaging is concentrated on the small irregular shaped particles.
In Fig. 2.11 a characteristic high-resolution image of the small, electron transparent
agglomerates is shown. Randomly oriented clusters of molybdenum oxide reveal lattice
fringes separated by characteristic distances of 0.34 nm and 0.37 nm. The whole area
depicted in Fig. 2.11 seems to be crystalline but it is clear that it is an agglomerate
rather than a single crystal.
The most active material in this family is produced from the ammonium containing
precursor. CO2 production sets in at 330 C. A decisive rise in activity is monitored at
420 C. At 450 C another plateau is reached and at 480 C a maximum in activity is
reached. The same material starts to produce acrolein at around 350 C. The activity is
rising with temperature only a small bend in the trace is observed at 370 C (Fig. 2.20,
Fig. 2.21, Fig. 2.22, Fig. 2.23).
0,00 0,05 0,10 0,15 0,20 0,25 0,300,5
256 30 C227 50 C232 70 C
Figure 2.14: pH trace of 256, 227, 232. Data normalised to
molybdenum and acid concentration respectively
The catalytic behaviour of the sodium containing hexagonal MoO3 is much lower.
However the first activity is registered at a quite low temperature 250 C. At 330 C and
at 350 C two local maxima are observed in a comparatively shallow trace. The
maximum activity is found at 480 C.
The potassium containing compound shows a very similar behaviour however the first
local maximum is more pronounced and the second one is missing.
2.3.4 Mo36O1128- supramolecular molybdenum oxide
The supramolecular compound is obtained with ammonia or with potassium as counter
ion. Usually low temperatures and high molybdenum concentrations need to be
employed (sample 256, 257, 228, 258, 225, 223, 249, 250, 245, 253, 246).
Using potassium as counter ion the supramolecular compound is obtained with K2MoO40.28 mol/l and HNO3 2.0 mol/l at 30 C, K2MoO4 yields the supramolecular compound
at 30 C and at 50 C the same is true when the acid concentration is increased to 5
Figure 2.15: A) HRTEM, 74; B) HRTEM, 74; C) SEM, 74, D) TEM, 74
Ammonia as counter ion (Fig. 2.14) yields the supramolecular phase when AHM 0.7
mol/l and HNO3 1 mol/l is used at 30 C. From a 1 mol/l AHM solution this phase is
precipitated at 50 C. Employing a 0.7 mol/l AHM solution and HNO3 2 mol/l
Mo36O1128- is obtained at 50 C.
Using the 0.28 mol/l K2MoO4 at 30 C the reaction starts at pH = 7. The titration curve
is similar to the one leading to hexagonal MoO3 with this concentration. However, in
this case much more acid is needed to reach the final pH. The titration curves of the 2
mol/l solution titrated with the 2 mol/l HNO3 start at pH = 7.5. The buffering regime at
around pH = 7 is quite extensive and roughly the same amount of acid is needed to
reach the final pH. The same shape is observed for the case 2 mol/l K2MoO4 5 mol/l
HNO3. The reaction at 30 C needs less acid than the one at 50 C to reach the final pH
With ammonia as counter ion (AHM 0.7 mol/l, HNO3 1 mol/l) the reaction starts at pH
= 5.3, the first buffering is less extensive and a comparatively big amount of acid is
used. In principle the same applies for the other reactions (Fig. 2.14 and 2.19).
100 200 300 400 500
Temperature / oC
Figure 2.16: TG-DSC of 256 and 228
The supramolecular compounds obtained all showed a variety of signals in the early 2
theta range, all similar to the original single crystal pattern from Bschen et al. . No
sample matched that pattern exactly; the differences in the powder patterns could arise
from different amounts of crystal water present in the precipitates.
In the potassium case one needs to distinguish among the products obtained from high
and from low concentrations. Whilst the low concentration product shows the 100 %
signal at 7 2 theta, the other products show various signals in this region and a 100 %
signal is difficult to determine (details Fig. 2.4).
The bands for the potassium-containing product are situated at 963, 882, 373 and 229
cm-1 for the low concentration product. Compared to that the bands for the high
concentration product are slightly shifted (961, 898, 372 and 240 cm-1). However the
differences in band shape and relative band intensities are even more decisive.
100 200 300 400 50090
Temperature / oC
Figure 2.17: TG-DSC trace of 250, 245 and 249
The ammonia-containing product shows bands at: 983, 959, 889, 372 and 234 cm-1.
This is in line with the bands reported in the literature. The samples show a large
variation in relative band intensities in the region assigned to the terminal Mo=O
stretching frequencies (Fig. 2.5).
Again small shifts depending on the counter ion are observed: 596, 658, 715, 818, 942,
967, 987, 1305, 1412, 1619, 3579 cm-1 (Fig. 2.9 and 2.10).
Looking at the NIR spectrum (Fig. 2.13) of the experiment carried out with the 2 (0.28)
mol/l K2MoO4 solution and the 2 (5) mol/l HNO3 it is to be seen that the compound
prepared at 50 (30)C shows in Table 2.5 the most intense water (NIR) bands at 1435
nm and at 1935 nm. The compound prepared at 30 C exhibits slightly smaller bands.
Band gap energies are is 3.30 eV and 3.30 eV. Switching from a 2 (0.28) mol/l acid
(K2MoO4) to a 5 mol/l the water (NIR) bands do not change their behaviour and are still
almost located at the same wavelengths. The band gap energy of both samples is found
at 3.43 eV.
0,0 0,2 0,4 0,6 0,8 1,0 1,2 1,4
10249 30 C219 50 C229 70 C250 30 C245 50 C244 70 C246 30 C246 50 C243 70 CpH
Figure 2.18: pH-trace 249, 219, 229; 253, 246, 243; 250, 245, 244.
Data normalised to molybdenum and acid concentration respectively
For the compound prepared from 0.7 and 1 mol/l AHM bands in the NIR region are
located at 1440, 1570, 1945, 2040 and 2150 nm. The first band, the third and the fourth
are assigned to a surface OH group the second to H2O and the last band is caused by
ammonia. The LMCT band is blue shifted from 316 to 308 nm with increasing AHM
concentration and the band gap energy is 3.46 eV (0.7 mo/l AHM) and 3.55 eV (1 mol/l
AHM) as shown in Table 2.5.
The supramolecular phase prepared at 30 C (0.28 mol/l K2MoO4, HNO3 2 mol/l) shows
only two sharp steps in the TG-trace (100 C, 322 C), the overall mass loss is around 8
% (Fig. 2.17). The DSC curve indicates three small exothermic peaks at 213 C, 286 C
and 355 C. At the endothermic signal and the shoulder in the 100 C region H2O and
OH is detected by MS. The occurrence of the first exothermic peak at 213 C is linked
with the evolution of OH and H2O. Between the two signals at 286 C and 355 C (at
344 C) a NOX signal is detected by MS.
When the same experiment (Fig. 2.17) is performed with a solution containing 2 mol/l
K2MoO4 the two supramolecular phases obtained at 30 C and at 50 C show almost
identical TG traces (overall mass loss 8 %). Water is removed at 100 C and this
coincides exactly with the appearance of the endothermic signal including the shoulder,
between 200 and 300 C a creeping mass loss is detected. Another peak assigned to
NOX in the MS is detected at around 340 C. After 350 C mass constancy was
0,0 0,1 0,20,5
5,5 227 50 C228 50 C225 50 C
Figure 2.19: pH trace, 227, 228, 225. Data normalised to
molybdenum and acid concentration respectively
achieved. The 50 C sample shows two distinct exothermic signals at 281 C and at 343
C. The gases evolved are the same as in the previous case and at the same
temperatures. The 30 C sample shows signals at the same positions but less distinct.
The same experiment is carried out only with a higher HNO3 concentration of 5 mol/l.
The TG-traces of the two supramolecular compounds are very similar to the ones
described in the preceding paragraph. However the total mass loss of the sample
prepared at 30 C is comparatively high: 12 %. The sample prepared at 50 C looses 10
% of its mass. Both samples show a broad endothermic DSC signal at 100 C where
water is released. At 130 C both samples show a sharp endothermic signal, which is
unrelated to any mass loss. At 278 C an exothermic mass loss is detected and only at
the endothermic signal at 340 C a final mass loss is observed setting NOX free.
The compound obtained from the AHM solution 0.7 mol/l shows an endothermic event
at around 100 C, when a large amount of water is removed from the sample (ca. 7 %).
After that a sequence of three exothermic events is registered at 279 C, 332 C and at
400 C. Each of them connected with a mass loss and at each of them water and NOx
are evolved. Total mass loss is 12 % (Fig. 2.16).
In a separate experiment samples were heated to the temperature of each event and then
the temperature was kept constant for one hour. After this the sample was investigated
200 250 300 350 400 450 500
Figure 2.20: TPRS first cycle; showing the effect of
counter ions in acrolein production
by Raman spectroscopy. It turned out that the supramolecular phase is transformed into
hexagonal MoO3 after the first exothermic event at 279 C. No change in phase is
observed after 332 C. At 400 C it transformed into orthorhombic MoO3.
A representative SEM image is shown in Fig. 2.15 C. The particles observed in the
SEM images are typically between 1 and 5 m and show an elongated shape with
facets. However, the facets are not perfect and some irregularities are observed. The
molybdenum to oxygen ratio is found to be close to constant over the sample by EDX
analysis (not shown here).
The SEM images reveal some smaller features (tenths of m). These features are more
visible in TEM images. In Fig. 2.15 D such an image is shown. The large somewhat
irregular shaped particles are observed in projection in the images. Moreover is the
carbon film covered with small (
lattice fringes encapsulated by amorphous/non-crystalline material. The lattice fringes
are separated with a characteristic distance of 0.37 nm.
The most active material prepared for this investigation is the supramolecular
compound (Fig. 2.22 and Fig. 2.23). Its CO2 trace is characterised by a rather sharp
local maximum at 230 C. Catalytic activity rises steeply at 380 C. Another
local maximum at quite high level is observed at 430 C. The highest overall
activity towards CO2 is seen at the end of the heating ramp.
Acrolein production starts at 380 C and no preceding local maximum is observed. At
430 C a turning point in the trace is observed. The maximum activity toward CO2 is
registered at the end of the heating ramp.
Figure 2.22: TPRS run first cycle; showing compounds prepared from
AHM starting material; oxygen conversion
200 250 300 350 400 450 5000
2.3.5 Up scaling
Preparation and pH-dependency
The hexagonal phase and the supramolecular phase were also synthesised in a 4 l
reactor in order to test the effects of up scaling. The pH curves of two supramolecular
samples that were precipitated in the different reactors under otherwise identical
conditions display a very similar behaviour up to pH = 3, further down the `small scale
sample showed an increased buffering region that can be associated with protonation
reactions. After the titration the `large scale sample was allowed to age, as mentioned
above. The Raman spectra showed identical positions for all major bands. XRD analysis
showed both the characteristic signal for the supramolecular phase at 7 degrees 2 theta,
but each sample showed a number of foreign signals.
Electron Microscopy and Electron Diffraction
Well-defined rods are observed in typical TEM images Fig. 2.11 of the hexagonal
material obtained by the up scaling experiments. The typical hexagonal rods are around
5 m in length and 0.5 m wide. Smaller agglomerates are observed as well in the SEM
images. However, the amount is much less than the amount observed in sample 227.
The mixture of big and small rods is clearly visible in TEM images such as Fig. 2.11.
The size of the big rod in Fig. 2.11 is 0.6 m times 4.3 m. The small rod located below
the big one in Fig. 2.11 has the dimension 50 nm times 400 nm, corresponding to a
volume approximately 1500 times less than the big rod. Lattice fringe imaging of the
suitable particles shows big (>50 nm) regular crystals. A typical example of such a
lattice fringe image is shown in Fig. 2.11. An FFT of the image is shown in Fig. 2.15.
The dominant lattice fringes are separated with distances of 0.61 nm and 0.36 nm,
respectively, in an angle of 70. The outermost 0.5-1 nm do not show the same lattice
fringes as the inner parts of the crystals.
The supramolecular particles obtained during the up scaling experiments (sample 74)
are more regular shaped for the large precipitation batch sample compared to the small
scale samples. This is observed in both SEM and TEM images. A characteristic TEM
image of sample 74 is shown in Fig. 2.11. Both large (>1 m) and small (
seems to be smaller and the shape better defined compared to sample prepared on a
HRTEM images of the smaller agglomerates found in sample 74 reveal randomly
oriented 3-5 nm clusters embedded in non-crystalline material as shown in Fig. 2.11.
The distance between the lattice fringes revealed in the clusters are found to 0.34 nm
and 0.37 nm. The clusters seem to be more well-developed in this sample than in the
small scale sample and the non-crystalline material less. Furthermore, larger (20-50 nm)
well-crystalline particles are observed in the sample Fig. 2.11. A Fourier Transform of
the crystal in shown in Fig. 2.15. The main features in the FFT correspond to lattice
fringe distances of 0.53 nm and 0.40 nm in an angle of 40. The outermost 0.5 nm of the
crystal shown in Fig. 2.11 is observed to be a different structure than the rest of the
Two samples prepared under similar conditions are compared (Fig. 2.24). In both cases
a 1 mol/l AHM stem solution was used and HNO3 1 mol/l. The large scale sample was
produced under preparative conditions including a 1 h aging time.
300 350 400 450 500
Figure 2.23: TPRS run first cycle; showing compounds prepared
from AHM starting material; acrolein production
Looking at the CO2 production the preceding local maximum is slightly shifted. Apart
from that the two traces match exactly until 250 C are reached. From that point on the
large scales trace is steeper and shows a marked plateau at 320 C. The overall
maximum is higher but reached at the same temperature. After that the activity towards
CO2 is declining. From 330 C onwards the two traces match again. During the second
cycle the activity is in the same range as at the end of the first one. However the activity
of the small scale sample is higher.
In the acrolein case the two traces match until the first maximum is reached. During the
constant temperature period the large scale sample is declining faster. In the second
cycle the range of activity is comparable to the end of the first one and again the small
scale sample is more active than the large scale.
0 60 120 180 240 300 360
large scalesmall scale
Figure 2.24: TPRS first and second cycle; showing the activity and
selectivity of the large scale sample and the small scale sample
Principally the herein described method allows producing four different families of
materials in a controlled manner. The assignment is based on integrative methods such
as Raman spectroscopy and XRD. TEM shows that every sample contains differently
sized and shaped particles with a high content of amorphous material. This is
particularly important to be considered for any efforts to derive structure activity
correlations. The presence of a non-uniform precipitate is easily understandable bearing
in mind the multitude of parallel reactions that occur during the titration. An earlier
Raman investigation already identified two independent reactions, more are likely. A
closer look at the Raman bands show identical band positions for each member of the
same family but different intensities, again indicating the presence of more than one
species. Another indicator for this is the band gap energies determined from the UV/Vis
experiments. This is most likely one of the reasons of many contradictions in the
literature concerning these materials.
500 750 1000 1250 1500 1750 2000 2250 2500-0.1
Figure 2.25: Spectroscopic characteristics NIR of orthorhombic
MoO3 . 251, 222 and 230
MoOx spectra show NIR bands with different intensities, distinguishable LMCT bands
and band gap energies (Eg) at RT. Based on the exact determination of such
spectroscopic characteristics the following LMCT bands (nm) (I) and Egs (eV) (II) are
attributed to the above mentioned MoOx families: (I) 312 (NH4+), 319 (K+); (II) 3.50
(NH4+), 3.43 (K+) to supramolecular Mo36; (I) 313 (NH4+), 312 (K+), 327 (Na+); (II)
3.35 (NH4+); 3.30 (K+), 3.27 (Na+) to hexagonal MoO3; (I) 296 (Li+); (II) 3.44 (Li+) to
orthorhombic MoO3 and (I) 284 (K+); (II) 3.77 (K+) to trimolybdate MoOx.
From a blue shift of the LMCT band in the series supramolecular/hexagonal
orthorhombic trimolybdate and a decreasing broadening of this band it may be
concluded that the cluster size decreases. All MoOx samples evolved NIR bands at
1435, 1940, and 2040 nm. They are assignable to an overtone mode of the OH
stretching vibration and a combination mode of the OH stretching and bending
vibration, respectively. Other NIR bands, e.g. those detected in MoOx samples prepared
from AHM at 1570 and 2150 are caused by ammonia.
1000 800 600 400 200
Supramolecular compound 257Hexagonal MoO
Intermediate 325 CIntermediate 340 COrthorhombic MoO
Raman shift [cm-1]
Figure 2.26: Raman investigation of TG post mortem samples at
2.4.1 Effect of counter cation
Despite the inhomogeneity mentioned above, this work has clearly shown the
considerable structure directing effects of counter cation. The influence of the counter
cation is based on its size and other properties such as activity and ionic strength. Whilst
only the big ions K+ and NH4+ caused spontaneous precipitation, the presence of Li+ and
Na+ required a heating period, leading to orthorhombic MoO3 in case of Li+ and to
hexagonal MoO3 in case of Na+. The latter structure was initially reported by Krebs[31;83]
and labeled as Mo5O16. Heating of K+ and NH4+ containing material yields either the
trimolybdate[43;78] or the hexagonal MoO3 whereas ammonia yields only supramolecular
or hexagonal MoO3, as reported.
In order to assess the thermodynamic stability of the four different families it is
assumed that there is the same general trend in solution and in solid material. Wienold
et al. carried out thermal decomposition of ammonium heptamolybdate. They
showed that in kinetically determined steps the system turned into hexagonal MoO3 and
subsequently into orthorhombic MoO3 at 350oC. The last step was identified as
thermodynamically favoured. If the formation of orthorhombic MoO3 is also
thermodynamically favourable in solution, the Na+, K+ and NH4+ counter cations
prevent such formation by precipitation of other intermediate phases. Formation of such
other phases would also be kinetically controlled, as also indicated by the large
temperature dependence. As Li+ is not able to force the precipitation of the hexagonal
phase because of its lower activity the orthorhombic phase is formed.
In order to address the question about the role of the counter cations during the
precipitation process Lehns definition of supramolecular chemistry as `chemistry
beyond the molecule intermolecular forces such as van der Waals forces, London
dispersion forces and hydrogen bonding becomes important. Further polarisability
introduced in the HSAB concept needs to be applied. It is likely that the comparatively
soft NH4+ could serve as an endo-template [85;86]. Fragments of the Octamolybdate will
group around the ammonia and interlink. As soon as the particle size is big enough and
a certain amount of species is formed, the solubility product is exceeded and
precipitation of the hexagonal MoO3 sets in. A retro synthetic approach corroborates
to this idea. Taking the ammonia inside the channel as a centre, only a few Mo-O-Mo
bridges need to be broken to yield these nanocluster building blocks. A comparable
mechanism should be possible with K+, taking into account that this ion is very similar
in size and ionic strength to ammonia. However K+ seems to be the limit for this
mechanism because under some experimental conditions (high Mo concentration, high
acid concentration, 70 C and spontaneous precipitation) the layered trimolybdate
structure is obtained. This trend is further followed as the smaller and harder ions Na+
and Li+ do not cause spontaneous precipitation, but rather hexagonal/ orthorhombic
MoO3 is formed after heating, as reported above. The smaller the ion the more difficult
it becomes to build up a stable spherical wrapping, consequently layered structures are
obtained from smaller ions and channel structures from bigger ones.
2.4.2 Effect of temperature and proton to molybdenum ratio
The obtained results show that temperature and the proton to molybdenum ratio are also
important control variables. 50 C is the most important boundary as the temperature
dependent investigations show. Therefore at this temperature most likely the reaction
mechanism is changing. High molybdenum concentrations and low temperature (30 C)
lead to a spontaneous precipitation of a supramolecular compound, which is very
similar to the Mo36O112 reported by Krebs. Low concentration and high temperature
leads to the formation of a hexagonal MoO3[79-81] the same structure is reported by
Krebs[83;87] and labelled as Mo5O16, orthorhombic MoO3 or trimolybdate depending on
the counter ion.
Up to pH = 3.5 the curves are identical and therefore the reaction mechanisms are alike.
This seems to be plausible because at this stage most likely protonation of the
heptamolybdate is taking place. This fits nicely to NMR data. At around pH = 3
where the reorganization to the Mo36O112 sets in, the 30 C curve is different to the other
curves. Octamolybdate is reported to be the dominant species [63;65;88] [44;68;89] in this pH
region. As transformation from octamolybdate into Mo36O112 requires many bonds to be
broken and reassembled by polycondensation reactions the slow down in the pH drop
seems plausible. At around pH = 2 another change in mechanism sets in. The 50 C
sample is acidified easily without yielding a precipitate. The 70 C moves parallel to the
30 C sample however at lower pH. It is likely that 50 C is not enough to overcome the
activation energy barrier to precipitate the hexagonal phase.
Using K2MoO4 as starting compound the coordination of the Mo is tetrahedral and the
experiment starts at higher pH. As the curves show the starting pH is a function of the
molybdenum concentration. As the first pH drop is very rapid the tetrahedral species is
not to be protonated. The first buffering region probably coincides with the formation of
a heptamolybdate species. Again this event depends on molybdenum concentration. The
following reaction pathway will be similar to the one described with ammonia as
counter ion. It is noteworthy that trimolybdate is only obtained with high molybdenum
and acid concentrations at higher temperatures.
According to Tytko the Mo36O112 is the major compound in solution at low pH and
precipitates as soon as the solubility product is reached. It is remarkable that the
connectivity has changed compared to the starting material. In the AHM precursor
only corner sharing octahedra are observed. In the Mo36O112 edge sharing connectivity
prevails and the pentagonal bipyramid as structural motif, which appears in catalytic
active material like Mo5O14, is formed[20;90;91]. Corner sharing also turns up in the
2.4.3 Effect of water
Krebs points out that Mo36O112 is only stable in the mother liquor. Water is responsible
for the hydrogen bonding which is probably the dominating coherent force in this
molecule. This phenomenon has been studied in detail in comparable
compounds[54;86]. As soon as water is removed the compound will decompose. This
explains the variation in XRD. Nevertheless the close similarity of the XRD to the
reference and the exact agreement of the Raman band positions corroborates to the idea
that the main structural motives prevail.
Investigating the reaction in the solid phase again the differences due to counter ions are
striking. Using ammonia as a counter ion, the final transformation is taking place at 50
C higher temperatures than in the potassium case. Therefore solid-state
thermodynamics are clearly influenced by the nature of the counter ion.
Moreover the phase transformation using ammonia as counter ion will be very different
because of the combustion of the ion. The large amount of water released at the first
exothermic event is probably to some extend related to this combustion. The same holds
true for the exothermic DSC signal. A good deal of heat is produced because of the
As NOx is released at 3 different temperatures showing three clearly distinguishable
DSC and MS peaks (water and NOx data not shown) it is probably situated in two
different places. At the first event the ammonia serving as linker between
supramolecular building blocks will be removed. After that ammonia is situated in the
channels of the hexagonal MoO3 and will only be removed at higher temperatures. The
last NO signal is detected with the K+ containing compounds as well. At this
temperature the NO3- that was brought into the solution by the nitric acid is removed.
As a mass loss is detected in this region as well it is very likely that the phase
transformation form the hexagonal phase to the orthorhombic MoO3 is related to a
removal of oxygen from the lattice or a further condensation. This idea is further
supported by traces of water that are also detected.
Comparing the supramolecular compound obtained with K+ as counter ion with the
ammonia containing compound it becomes clear that the first transformation is also a
condensation step. The water being released in this step by the K+ containing compound
cannot originate from a combustion process but from polycondensation. In this respect
solid phase and aqueous chemistry run parallel because some activation barrier needs to
be overcome to induce this process.
The similarities between the supramolecular phase and the hexagonal MoO3 become
very clear when the sample prepared from a 2 mol/l K2MoO4 solution is compared to
the sample prepared from a 0.28 mol/l K2MoO4 solution. Mass loss and DSC trace are
very similar. Therefore only the condensation process will vary slightly.
The water contents can be estimated from the NIR bands and from the TG-MS results
for the Li+, Na+ and K+ containing precursors. Compounds, which show a big mass loss,
always have marked water bands. This correlation is not possible for the ammonia
containing samples because the water and ammonia vibrations are combined.
The XRD pattern of the orthorhombic MoO3 obtained from Li2MoO4 shows broad
signals and a comparatively high background indicating low crystallinity. One reason
for this is that the degree of polymerisation due to a condensation in water at the chosen
conditions is too low to form big crystalline particles or the solubility product is reached
too early. DSC and TG-MS clearly shows an ongoing polycondensation.
The sample prepared at 50 C shows the biggest overall mass loss concerning water.
However the first step where only associated water is removed is biggest as well. One
reason for this is probably a high degree of protonation at the outer shell of the
polymeric precursor in solution being a good docking place for hydrogen bonding to
water molecules. Assuming that the second step is the water from the polycondensation
process the 50 C sample looses 2.9 % in this step. For the 30 C sample the same
amount is calculated. Only for the 70 C sample 3.2 % are calculated. Therefore in this
sample more OH groups suitable for further condensation were created. Again a change
in the reaction mechanism can be established.
Taking all these results together it can be concluded that at higher temperatures in
solution the sites for protonation are changing and protonation is much more efficient.
This idea is corroborated by the above described changes in the pH curves of the
ammonia containing samples as a function of temperature.
2.4.4 Structure determination by XRD and TEM
Phase characterisation of materials by XRD is widely used. However, such integral
techniques are insufficient to reveal the detailed local phase- and structure
determination, which might be relevant for the purposes of the studied material,
especially in catalysis. Lattice fringe images of sample 130, such as Fig. 2.11 show
well-developed crystals, from which the relevant lattice plane distances can be
measured. Several high-resolution images revealing lattice fringes acquired from sample
130 are analysed, and the measured lattice plane distances are compared with the
corresponding XRD pattern. This is shown in Fig. 2.15 C. The XRD shows narrow
distinct peaks coinciding with diffraction peaks calculated from the model structure of
hexagonal molybdenum trioxide. The signal to noise ratio is very high and no additional
features are observed between the well-defined peaks. The observed lattice plane
distances measured in the high-resolution images are marked under the XRD pattern in
Fig. 2.15 C. HRTEM images cannot and should not be used quantitatively, so the
comparison is done qualitatively. Several lattice plane distances observed in the
HRTEM images are not revealed in the XRD, indicating that the HRTEM images are
acquired of crystalline structures which are not resolved by the integral technique of
XRD. In Fig. 2.11 both a very big particle and a small particle are observed. The
volume of the bigger particle is approximately three orders of magnitude larger than the
volume of the smaller one. The XRD technique is volume sensitive and hence the
structure of the largest volume is favoured in the XRD. The diffraction pattern of the
structure of the smaller crystals is suppressed by the diffraction pattern of the large
volume of big well-defined crystals in the sample. The local structure of the smaller
particles in the sample might be highly relevant for the resulting structure of the active
catalysts, and should not be neglected. In order to validate the comparison between X-
ray diffraction and diffraction of electrons in the sample, diffraction simulations are
performed using X-rays and electrons. The simulated powder diffraction spectra of the
hexagonal molybdenum trioxide model reveal exactly the same features for electron
diffraction and X-ray diffraction, although slight changes in the intensities are observed.
The morphology of the biggest particles in the samples shows clear differences in the
two families (hexagonal and supramolecular). The regular hexagonal rods with well-
Figure 2.27: A FFT of 74, B FFT of 130, Comparison electron diffraction
versus X-ray diffraction
defined facets observed in Fig. 2.11 are a further indication of the single crystalline
hexagonal atomic structure of biggest particles in sample 227. The more irregular
morphology of the largest particles observed in Fig. 2.11 might indicate a more
complicated atomic structure or the fact that the biggest particles in the small scale
sample are agglomerates of smaller crystals.
In the following the crystallographic structure of the studied samples will be discussed
on the basis of the lattice fringe images acquired from area of the sample, which are
electron transparent, i.e. thin agglomerates.
The samples precipitated in the small-scale set-up consist of randomly oriented clusters
in the 3-5 nm scale, as shown in Fig. 2.11. The fact that lattice fringes are revealed